Blended Cements Produced with ... - Materials Science
Embed Size (px)
Transcript of Blended Cements Produced with ... - Materials Science
ISSN 1392–1320 MATERIALS SCIENCE (MEDŽIAGOTYRA). Vol. 21, No. 1. 2015 Blended Cements Produced with Synthetic Zeolite Made from Industrial By-Product Danutė VAIČIUKYNIENĖ 1 ∗, Vitoldas VAITKEVIČIUS 1, Aras KANTAUTAS 2, Aurelijus KARTOVICKIS 1, Žymantas RUDŽIONIS 1 1 Faculty of Civil Engineering and Architecture, Kaunas University of Technology, Studentų str. 48,
LT-51367 Kaunas, Lithuania 2 Faculty of Chemical Technology, Kaunas University of Technology, Radvilėnų Rd. 19, LT-50254 Kaunas, Lithuania
Received 06 November 2013; accepted 22 February 2014
Zeolites are appropriate supplementary cementitious materials in cement and concrete industry. In the present work synthetic zeolites were used as supplementary material in hardened cement paste and some properties as well as its influence on Portland cement hydration was determinate. X-ray powder diffraction, scanning electronic microscopy and energy-dispersive X-ray spectroscopy, FTIR spectroscopy were used as investigation methods. The compressive strength of hardened cement paste was measured at day 3, 28 and 60. The instrumental analysis showed that zeolite A(Na) dominates and unreacted Al(OH)3 remains in the investigated synthetics zeolites, made from thermal and mechanical treated AlF3 production waste. The Chapelle test showed that both zeolites have good pozzolanic properties. The samples compressive strength remained close to the control samples compressive strength, reducing the amount of Portland cement, i. e., changing it by zeolite. After 60 days, the compressive strength was the best in the samples where 5 % of Portland cement was replaced by the synthetic zeolite. The compressive strength of the samples increased by 9 % compared with control samples. This research provides a real opportunity to save cement thus disposing the waste. Keywords: blended cements, synthetic zeolite, by-product.
Various minerals are often incorporated in Portland cement composition including zeolites [1 – 3], additives improving the characteristics of the resulting product manufacturing composite building materials. Scientists C. Karakurt and I. B. Topcu  found that the natural zeolite pozzolanic activity is higher than amorphous, natural pozzolanic materials pozzolanic activity. Concrete strength increased, while the zeolite reduced chloride penetration and corrosion of concrete having used only 15 % of natural zeolite. The samples with zeolite shrinkage deformations were lower in comparison with control samples.
Studying the pozzolanic additives (natural zeolite, fly ash, blast furnace slag) influence on the concrete properties (its alkali corrosion, resistance to high temperatures and sulphates) the researchers [5, 6] found that at high temperatures, ash additive reduces sample tension strength loss and cracks appearance. Concrete strength increases due to the pozzolanic reactions with portlandite. Length variations and micro-structure research, compared with the usual CEM I 42.5 showed that the building blends with different additives reduce the alkaline corrosion probability and increases the resistance to sulphates.
Also, natural zeolite (clinoptolite) was used as filling and bubble-generating additive in the manufacturing aerated concrete . Test results showed that the burnt zeolite can perform both the function of filling and bubble-
∗Corresponding author. Tel.: +370-37-300465; fax.: +370-37-300454. E-mail address: [email protected] (D. Vaičiukynienė)
generating agent. Also, it is not necessary to use aluminum powder in the cement production, and its compressive strength reaches up to 4.6 MPa and density – 930 kg/m3.
Modified zeolite additive can increase the strength and durability of concrete at its optimal amount is between 0.6 % and 1.0 % . Concrete absorption improves regardless of the cement and mixture ratio in the mixture, and concrete water permeability improves having added 30 % of fly ash. It was concluded that the most effective to use the composite mixtures of fly ash and zeolite.
The ultrasonic transmission rate also increases increasing the amount of zeolite in mixture, but the Young's modulus, compressive and bending strength decreases . The research results showed that the zeolite can be used as a filling, but not as a substitute for cement, as during the tests on the fresh concrete paste replacing up to 30 % of cement by zeolite it was found that it improves the dough resistance to delamination. Rapid chloride penetration test (RCPT) curves at solid state, replacing up to 30 % of the cement, showed lower values and higher surface resistance .
The research of natural zeolite rocks and Ca(OH)2 solution pozzolanic activity by conductometry power method  stated that the zeolite rock has a large pozzolanic activity. These results have also described the direct zeolite dispersivity dependence on mechanical and pozzolanic properties.
Although natural zeolite with silica fume and ash is pozzolanic material, however it more influences the strength of the mixture in compound cement dough with a lower water and cement ratio. However in the cement dough with a bigger water/cement ratio and the lower
replaced part of the zeolite by cement, hydration reaction takes place better .
The calculation of composite zeolite cement hydration rate solidification for 360 days and their hydration products, it was concluded that zeolite additive in mixture during hydration reacted with Ca(OH)2 and made cement hydration products . Pozzolanic reaction of zeolite in the first days was slow, but it became much faster after 28 days of hydration.
Th. Perraki investigated the influence of natural zeolite to cement hydration. Tested zeolite from “II type of heulandite” had a considerable pozzolanic activity of 0.555 g Ca(OH)2 per gram of zeolite (according to Chepelle methodology). During hydration time a larger quantities of Ca(OH)2 are bounded having inserted this zeolite into dough and the compounds similar to cement hydration compounds are produced .
The literature data show that natural zeolites are promising pozzolanic additive. Therefore, this work investigates artificial zeolites derived from highly contaminated with fluorine compounds amorphous SiO2 the use capabilities in cement systems.
2. MATERIALS AND METHODS
2.1. Raw materials
The Portland cement CEM I 52.5 R (specific surface is 370 m2/kg, paste of normal thickness 27.3 %, the initial setting time is 130 min, final setting is 215 min) was used in this study.
Fig. 1. X-ray diffraction pattern of AlF3 production waste. Notes:
A – AlF3 · 3.5H2O
Table 1. The element composition of AlF3 production waste
Element Wt, % At, %
Oxygen 41.98 52.09
Aluminum 2.98 2.19
Silicon 33.43 23.64
Fluorine 20.84 21.79
Calcium 0.30 0.15
Iron 0.46 0.16
Total 100 100
Reagents NaOH (DeltaChem, Czech Republic), Al(OH)3 (Lachema, Czech Republic), industrial by-product, i. e., amorphous SiO2 · nH2O (Lifosa, Lithuania), as silica and alumina source were used in the synthesis of
zeolites. According to the X-ray diffraction curves (Fig. 1) there are amorphous SiO2 · nH2O (rise from 10 up to 30°) and crystalline AlF3 · 3.5 H2O.
Very high fluoride concentrations were obtained after the amorphous silica elemental analysis (Table 1). It is believed that fully unreacted H2SiF6 in investigated silica should be left in addition to these compounds. The determination of H2SiF6 in heterogeneous systems is problematic.
2.2. Experimental techniques The X-ray powder diffraction data were collected with
DRON-6 X-ray diffractometer with Bragg-Brentano geometry using Ni-filtered Cu Kα radiation and graphite monochromator, operating with the voltage of 30 kV and emission current of 20 mA. The step-scan covered the angular range 2° – 70° (2θ) in steps of 2θ = 0.02°.
The structure of hardened cement paste was studied by scanning electronic microscopy. A high resolution scanning electron microscope FEI Quanta 200 FEG with a Schottky field emission gun (FEG) was used. The quantitative analysis was carried out with the energy-dispersive X-ray adapted to the SEM for microanalysis. An energy-dispersive X-ray spectrometer (EDS) has a silicon type drift droplet detector.
The cement paste hydration temperature measurements were performed with 8-channel USB TC-08 Thermocouple Data Logger (temperature measurement range from –270 °C to +1820 °C).
The pH was determined by a Premium Aquatics Supplies Hanna HI-98129 tester, which simultaneously measures aqueous pH and temperature. Range pH is from 0.00 to 14.00 pH.
IR spectra were recorded with Perkin Elmer FT-IR System spectrometer. For the IR analysis, 1 mg of the substance was mixed with 200 mg of KBr and compressed in a forming press under vacuum.
Zeolites have been produced by using mechanical treatment, by grinding in the laboratory ball mill (grinding bodies – steel balls), or by heating a suspension in kiln SNOL 200/200.
Constant flow was stable and the content of the modified zeolite addition was 0; 5; 10 and 15 % mass in all test samples. Water and cement ratio (V/C = 0.40) was constant in all samples. The formed test samples (2×2×2 cm size cubes) were hardened for 3, 28, and 60 days. The compressive strength of hardened cement paste was measured by EN 196-1.
3. RESULTS AND DISCUSSION
3.1. Zeolitization of AlF3 production waste Na2O : Al2O3 : SiO2 : H2O molar ratio equal to
1.5 – 2 : 1 : 2 : 10 was taken for AlF3 production waste zeolitization. This ratio is the most optimal to get the synthetic zeolite A, which is widely used [15, 16].
The initial dry matter was thoroughly mixed until homogenous; then pouring the required amount of water it was stirred until a homogeneous liquid suspension. In the first case, it was heat-treated by heating a suspension for four hours at 110 °C (hereinafter referred to as 1-zeolite),
Fig. 2. SEM images and element of composition of synthetic zeolites. Notes: a – 1-zeolite; b – 2-zeolite
and in the second case, mechanically grinding it for 15 minutes in vibro mill (hereinafter referred to as 2-zeolite). 15 min duration is optimal based on previous work .The excess amount of sodium hydroxide in the obtained zeolites was washed with water to neutral pH medium. The product was dried at 80 °C in 24 hours.
Both zeolite samples were examined by scanning electron microscopy (Fig. 2). SEM images show that 1-zeolite obtained during the process of AlF3 production waste zeolitization for four hours at the temperature of 110 °C (Fig. 2, a) crystals have a cubic character, and zeolitizing AlF3 waste mechano-chemically (grinding in vibro mill 15 min) (Fig. 2, b) besides to cubic crystals, characteristic to zeolite A there are particles of not defined form, which yet have not fully recrystallize to crystalline zeolite.
EDS analysis showed that silicon, aluminum, and natrium dominated in both synthetic zeolites. Natrium concentration was managed to reduce up to 2.62 % by washing 2-zeolite with water, while 5.58 % natrium remained in 1-zeolite.
According to the X-ray diffraction curves of synthetic zeolites (Figure 3), zeolite A (Na) (d: 1.231, 0.870, 0.710, 0.410, 0.371, 0.328, 0.262 nm) dominate and there are also not completely unreacted Al(OH)3 (d: 0.485, 0.438, 0.433, 0.234 nm).
Infrared IR spectra can provide valuable information in study of the material structure difference. IR curves (Fig. 3, b) of analyzed zeolites had a large number of absorption bands in (400 – 4000) cm–1 range. Zeolites structure peculiarities are determined according to (1100 – 400) cm–1 zone. The characteristic absorption bands for Zeolite A  are: (1000 – 1091) cm–1 in the range of asymmetric valence fluctuations, 765, 791, and 704, 660 cm–1 in the range of symmetric valence fluctuations, 573, 555 cm–1 in the range of double shell rings fluctuation and 471, 489 cm–1 in the range of Si(Al)–O deformation vibration.
The absorption bands in 2-zeolite spectrum 3616, 3516, 3451, 961, 734, 660 cm–1 are assigned to gibbsite (Al(OH)3), i. e., to initial material, which remained unreacted. The received FT-IR analysis results agree well with the research results of other scientists [19 – 21].
Fig. 3. X-ray diffraction patterns (a) and FT-IR spectra (b) of synthetic zeolites: 1 – 1-zeolite; 2 – 2-zeolite; G – gibbsite Al(OH)3; Z – zeolite A Na96Al96Si96O384 · 16H2O
3.2. Pozzolanic activity of 1-zeolite and 2-zeolite Zeolites can be used as a pozzolanic material
according to ENV 197-1 directive. Mixed with water, zeolites do not harden like most other pozzolanic materials, but zeolites begin to react with soluble calcium hydroxide (in the water), if they are very finely granulated at normal i. e., at room temperature; calcium silicates and calcium aluminates, determining the strength of the concrete  is the result of this process.
After Chepelle test  it was found that 2-zeolite bound almost the same amount of calcium hydroxide (0.9751 g ±0.01 g Ca (OH)2/g zeolite) as well as 1-zeolite (0.9633 g ±0.01 g Ca (OH)2/g zeolite), so both zeolites can be attributed to pozzolanic materials group.
Fig. 4. X-ray diffraction patterns of pozzolanic reaction product.
Notes: 1 – 1-zeolite; 2 – 2-zeolite. F – (Na2Ca)0.075 (Al0.3Si0.7)O2(H2O)0.22; H – hydrocalumite – Ca2Al(OH)7· ·3H2O; R – hydrogarnet – Ca3Al2(O4H4)3; G – gibbsite Al(OH)3; C – calcite CaCO3; K – calcium silicate hydrate Ca1.5SiO3.5·H2O
X-ray analysis of pozzolanic reaction products (solids) showed that sodium calcium alumohydrosilicates (Na2Ca)0.075(Al0.3 Si0.7)O2(H2O)0.22, calcium aluminate
hydrate (hydrocalumite) Ca2Al(OH)7 · 3H2O; gibbsite Al(OH)3 and calcium silicate hydrate Ca1.5SiO3.5H2O in 1-zeolte (Fig. 4, curve 2) formed after the pozzolanic reaction. 2-zeolite in reaction with calcium hydroxide formed calcium aluminate hydrates (hydrogranates) Ca3Al2(O4H4)3; gibbsite Al(OH)3, calcite CaCO3 and calcium silicate hydrate Ca1.5SiO3.5H2O.
3.3. Synthetic zeolites in cement systems
Portland cement clinker mineral hydration reactions are relatively slow. Their rate depends on many factors, including nature and quantity of the cement additives. It is convenient to follow the progress of these reactions according to solidifying samples temperature change kinetic curves (Fig. 5). Hydration maximum temperature of cement sample when 5 % of 1-zeolite is modified Portland cement (Fig. 5, a) increases by 3 degrees (up to 58 °C) compared with the control – free of zeolite – sample hydration temperature (55 °C). Hydration temperature drops to 50 °C and 48 °C C taking its larger quantities (10 % and 15 %).
Analogous tendencies are observed using 2-zeolite (Fig. 5, b) also. Hydration maximum temperature of cement sample with 5 % of 2-zeolite amount is higher than the control sample, and the temperature of these samples was similar to controls inserting into the cement increased by 10 % and 15 % 2-zeolite amount. However, any investigated amount of 1-zeolite and 2-zeolite decreases the initial setting of cement paste (the maximum of temperature moves to longer duration area).
The compressive strength of the samples after three days of hydration remained close to the control samples strength (Fig. 6). The highest compressive strength in tested conditions after 28 days had the samples containing 5 % of 1-zeolite, changing Portland cement to 1-zeolite in different quantities. So, the zeolite of pozzolanic properties displays not immediately; they become apparent after longer hydration time, i. e., only after 28 days. Zeolite reacting with calcium hydroxide composes secondary hydration products, the pores and capillaries in cement stone as hydraulic additives.
After 60 days, the best compressive strength had the samples, which were formed replacing Portland cement by 2-zeolite. Taking 5 % of this zeolite, the samples compressive strength increased by about 9 % compared with the control (Fig. 6, b).
X-ray diffraction analysis results of the hydrated samples (Fig. 7) show that calcium hydrosilicate, alite, belite, portlandite and calcite, as well as small amount of vaterite and gibbsite dominated in the cement stone with 1-zeolite. Calcium silicate hydrates, alite, and belite also prevail in the samples with 2-zeolite.
In both cases portlandite peak in the X-rays diffraction patterns decreases increasing the amount of zeolite. It can be concluded that the replacement of Portland cement binds portlandite to secondary calcium silicate hydrates during the hydration.
Microstructure of cement stone is given in SEM pic-tures (Fig. 8). Hexagonal calcium (sodium) silica alumina hydrate (Fig. 8, a) are formed in cement stone when Portland cement is replaced by 15 % of 1-zeolite. The EDS
Fig. 5. Cement paste hydration process temperature dependence on the quantity of portlandcement supplementary material: a – 1-zeolite; b – 2-zeolite
Fig. 6. Compressive strength of hardened cement paste after 3, 28 and 60 days with 0, 5, 10 and 15 % of portlandcement supplementary
material : Z1 – 1-zeolite; Z2 – 2-zeolite
Fig. 7. X-ray diffraction patterns of hardened cement paste after 28 days hydration with 0 % (1); 5 % 1-zeolite (2); 10 % 1-zeolite (3);
5 % 2-zeolite (4) and 10 % 2-zeolite (5) of portlandcement supplementary material. Notes: CC – calcite; G – gibbsite; CH – portlandite; K – calcium hydrosilicate; V – vaterite; A – alite; D – belite
Fig. 8. The SEM images of hardened cement paste: with 15 % 1-zeolite (a) and with 15 % 2-zeolite (b). The elemental composition of point A (c). Notes: CH – portlandite; K – calcium hydrosilicate; F – calcium silica alumina hydrate
results reveal that those crystals are calcium aluminosilicate hydrate and its elemental composition is shown in (Fig. 8, c). Similar crystals are reported in studies [22, 23]. Hexagonal tabular Ca(OH)2 crystals and small,
semi-amorphous calcium silicate hydrates needle crystals can also be identified in these pictures. Very detailed semi-amorphous microstructure can be seen in the SEM photos of the samples with 2-zeolite. The newly formed calcium silicate hydrates of CSH (I) type form small needle crystals (Fig. 8, b).
The obtained results shows that the most purposeful is to replace 5 % of Portland cement with 2-zeolite in cement mixture.
The instrumental analysis (X-ray diffraction, IR spectroscopy, SEM) showed that zeolite A(Na) dominates and unreacted Al(OH)3 remains in the investigated synthetics zeolites, made from thermal and mechanical treated AlF3 production waste. 1-zeolite crystals have a cubic shape and there are particles of smaller and uncertain form in 2-zeolite near the cubic crystals, characteristic to zeolite A. The Chapelle test showed that both 1-zeolite and 2-zeolite have good pozzolanic properties.
By using 5 % of investigated zeolites the hydration temperature maximum of cement pastes, increases by 3 degrees (up to 58 °C) compared with the hydration temperature (55 °C) of reference sample. Hydration temperature drops down to 50 °C and 48 °C taking 1-zeolite larger quantities (10 % and 15 %). By using the larger quantities (10 % to 15 %) of 2-zeolite hydration temperature was close to the reference sample temperature. However, any investigated amount of 1-zeolite and 2-zeolite decreases the initial setting of cement paste (the maximum of temperature moves to longer duration area).
The samples compressive strength remained close to the control samples compressive strength, reducing the amount of Portland cement, i. e., changing it by zeolite. After 60 days, the compressive strength was the best in the samples where 5 % of Portland cement was replaced by the 2-zeolite. The compressive strength of the samples increased by 9 % compared with control samples. The increase of sample strength can be explained by the fact that enclosed zeolite during hydration binds portlandite to the secondary calcium silicate hydrates. This research provides a real opportunity to save cement thus disposing the waste.
1. Caputo, D., Liguori, B., Colella, C. Some Advances in Understanding the Pozzolanic Activity of Zeolites: The Effect of Zeolite Structure Cement and Concrete Composites 30 (5) 2008: pp. 455 – 462. http://dx.doi.org/10.1016/j.cemconcomp.2007.08.004
2. Narasimhulu, K., Gettu, R., Babu, K. Beneficiation of Natural Zeolite through Flash Calcination for Its Use as a Mineral Admixture in Concrete Journal of Materials in Civil Engineering 10 2013: pp. 1061 – 1069.
3. Ramezanianpour, A. A., Kazemian, A., Sarvari, M., Ahmadi, B. Use of Natural Zeolite to Produce Self-consolidating Concrete with Low Portland Cement Content and High Durability Journal of Materials in Civil Engineering 25 (5) 2012: pp. 589 – 596.
4. Karakurt, C., Topcu, I. B. Effect of Blended Cements with Natural Zeolite and Industrial By-products on Rebar Corrosion and High Temperature Resistance of Concrete
Construction and Building Materials 35 2012: pp. 906 – 911.
5. Najimi, M., Sobhani, J., Ahmadi, B. An Experimental Study on Durability Properties of Concrete Containing Zeolite as a Highly Reactive Natural Pozzolan Construction and Building Materials 35 2012: pp. 1023 – 1033.
6. Karakurt, C., Topcu, I. B. Effect of Blended Cements Produced with Natural Zeolite and Industrial By-Products on Alkali-Silica Reaction and Sulfate Resistance of Concrete Construction and Building Materials 25 (4) 2011: pp. 1789 – 1795.
7. Karakurt, C., Kurama, H., Topçu, I. B. Utilization of Natural Zeolite in Aerated Concrete Production Cement and Concrete Composites 32 (1) 2010: pp. 1 – 8.
8. Ikotun, B. D., Ekolu, S. Strength and Durability Effect of Modified Zeolite Additive on Concrete Properties Construction and Building Materials 24 (5) 2010: pp. 749 – 757.
9. Kılınçarslan, Ş. The Effect of Zeolite Amount on the Physical and Mechanical Properties of Concrete International Journal of the Physical Sciences 13 (6) 2011: pp. 3041 – 3046.
10. Ramezanianpour, A., Kazemian, A., Sarvari, M., Ahmadi, B. Use of Natural Zeolite to Produce Self-Consolidating Concrete with Low Portland cement Content and High Durability Journal of Materials in Civil Engineering 25 (5) 2013: pp. 589 – 596.
11. Rosell-Lam, M., Villar-Cociña, E., Frías, M. Study on the Pozzolanic Properties of a Natural Cuban Zeolitic Rock By Conductometric Method: Kinetic Parameters Construction and Building Materials 25 (1) 2011: pp. 644 – 650. http://dx.doi.org/10.1016/j.conbuildmat.2010.07.027
12. Poon, C. S., Lam, L., Kou, S. C., Lin, Z. S. A Study on the Hydration Rate of Natural Zeolite Blended Cement Pastes Construction and Building Materials 13 (8) 1999: pp. 427 – 432.
13. Kontori, E., Perraki, T., Tsivilis, S., Kakali, G. Zeolite Blended Cements: Evaluation of Their Hydration Rate by Means Of Thermal Analysis Journal of Thermal Analysis and Calorimetry 96 2009: pp. 993 – 998.
14. Perraki, Th., Kakali, G., Kontoleon, F. The Effect of Natural Zeolites on the Early Hydration of Portland Cement Microporous and Mesoporous Materials 61 (1 – 3) 2003: pp. 205 – 212.
15. Fernandes Machado, N. R. C., Malachini Miotto, D. M. Synthesis of Na–A and–X Zeolites from Oil Shale Ash Fuel 84 (18) 2005: pp. 2289 – 2294.
16. Cundy, C. S., Cox, P. A. The Hydrothermal Synthesis of Zeolites: History and Development from the Earliest Days to the Present Time Chemical Reviews 103 (3) 2003: pp. 663 – 702.
17. Vaitkevičius, V., Šerelis, E., Lygutaitė, R. Production Waste of Granite Rubble Utilization in Ultra High Performance Concrete Journal of Sustainable Architecture and Civil Engineering 2 (3) 2013: pp. 54 – 60.
18. Brek, D. Zeolite Molecular Sieves. Moscow: Mir, 1976: pp. 27, 56, 58, 99 – 103, 282, 288 – 291. 781 p. (in Russian).
19. Musyoka, N. M., Petrik, L. F., Hums, E., Baser, H., Schwieger, W. Ultrasonic Monitoring of Zeolite. A Crystallization from Coal Fly Ash Catalysis Today 190 2012: pp. 38 – 46.
20. Gougazeh, M., Buhl, J.-Ch. Synthesis and Characterization of Zeolite a By Hydrothermal Transformation of Natural Jordanian Kaolin Journal of the Association of Arab Universities for Basic and Applied Sciences http://dx.doi.org/10.1016/j.jaubas.2013.03.007. 2013: pp. x – x+8. http://dx.doi.org/10.1016/j.jaubas.2013.03.007
21. http://www.natural-zeolite.com/downloads/zeolite-in-cement.pdf. [Žiūrėta: 2013-10-30].
22. Payá, J., Monzó, J., Borrachero, M. V., Velázquez, S., Bonilla, M. Determination of the Pozzolanic Activity of Fluid Catalytic Cracking Residue. Thermogravimetric Analysis Studies on FC3R-Lime Pastes Cement and Concrete Research 33 (7) 2003: pp. 1085 – 1091. http://dx.doi.org/10.1016/S0008-8846(03)00014-0